## Solution Processability and Thermally Activated Delayed Fluorescence: Two Steps towards Low-Cost Organic Light Emitting Diodes

## Sahadev Somasundaram

School of Chemical Engineering, The University of Queensland St. Lucia, QLD 4072, Australia d.somasundaram@uq.edu.au

## Abstract

Organic Light Emitting Diodes (OLED) have experienced vast attention in the scientific literature as the leading contender for the next generation of electronic lighting technology. However, while research continues to push the limit for OLED performance and efficiencies, minimal attention is paid to the processability and suitability for mass production. In this regard, Solution Processability (SP)  and  Thermally  Activated  Delayed  Fluorescence  (TADF)  in  OLEDs  are  two  recent  discoveries which have significantly improved the capacity for low-cost processing without compromise to their performance efficiencies. This meta-analysis is focused on these discoveries and their application to OLEDs. Recent peer-reviewed studies of OLEDs employing both SP and TADF are reviewed in order to highlight physical fundamentals and discover synergistic effects when incorporating both factors into a single OLED device. Additionally, some other recent trends targeting efficient manufacturing of OLEDs are identified, and logical future directions for interested researchers are discussed.

Keywords:  Organic  light  emitting  diode;  solution  processable;  thermally  activated  delayed fluorescence; OLED; TADF; organic semiconductor.

## Introduction

Organic light emitting diodes (OLED) are expected to serve as the next generation of technology for electronic  lighting  and  display  applications.  While  not  yet  sufficiently  developed  for  broad commercialisation,  OLEDs  are  beginning  to  show  superior  performance  to  their  inorganic counterparts - in fact, several global electronics developers have opted for OLED-based displays in their product lines. The organic materials used in OLEDs carry added versatility in that they can maintain complete opto-electronic function when deposited onto flexible plastics or even fabrictype  substrates.  Furthermore,  the  underlying  organic  molecular  structure  allows  for  endless possibilities in tailoring production and performance efficiencies through unique molecular designs. Finally,  recent  research  has  focused  on  two  inherent  properties  that  dramatically  improve production efficiency, which are only available to organic materials: Thermally Activated Delayed Fluorescence (TADF) and Solution Processability (SP).

The first notable demonstration of TADF by Chihaya Adachi and collaborators in 2012 [1] essentially quadrupled the possible performance efficiencies of conventional fluorescent OLEDs. By utilising a phenomena formerly termed 'E-type delayed fluorescence' [2], the group discovered that purely organic materials can harness light emission from triplet-state excitons otherwise only accessible to materials containing expensive heavy metals. Thus, TADF materials not only improve the efficiency of  conventional  OLEDs  but  reduce  the  production  cost  by  eliminating  the  need  for  expensive materials. Since discovery, most  TADF  studies  have  focused  on  achieving greater device performance through innovative molecular design. Over the previous few years, several reports have demonstrated achieving near 100% Internal Quantum Efficiency (IQE) [3,4], as well as External Quantum  Efficiency  (EQE)  higher  than  the  most  promising  phosphorescent  OLEDs  [5,6].  As  a consequence, the production efficiency, or the ability to be manufactured at the commercial scale with minimal cost, receives considerably less attention. Studies of TADF-based materials and devices are widespread throughout the scientific literature; the mechanisms and significance of TADF are explained in numerous reviews, books and articles [1,7-14], and are thus not discussed here.

Solution processing is significantly cheaper than the typical vacuum-based deposition techniques, which require expensive equipment and a high resource cost per unit area of deposited material. Solution processing techniques also require less technical expertise for operation, are more suitable for large-scale depositions and are compatible with the existing roll-to-roll (R2R) processes used for mass production of thin-film semiconductors. Solution processing occurs from a solution of the deposition  materials  dissolved  in  a  solvent,  which  is  to  be  evaporated  through  the  deposition process.  It  should  be  noted  that  while  solubility  is  considered  a  major  advantage  of  organic semiconductor materials, not all such materials are equally, or even sufficiently, soluble in suitable solvents; thus, solubility is a critical property when evaluating materials for solution processing. High solubilities are often associated with a greater presence of alkyl and alkoxyl moieties and a longer aliphatic chain [15]; this is typically seen in polymers. Higher solubility will i) result in a more uniform and homogeneous film morphology, removing the potential for charge trapping; and ii) allow a more uniform  distribution  of  dopants  in  host:dopant  complex  films,  resulting  in  a  lower  chance  of concentration quenching [16] and aggregation-caused quenching [17,18].

Many  industrial  reports  and  popular  science  articles  recognise  that  despite  the  exceptional performance  of  modern  OLEDs,  the  cost  involved  with  manufacturing  is  preventing  them  from dominating the electrical lighting and electronic display markets. It is believed that the key to these manufacturing issues lies in breakthroughs of the fundamental physics and chemistry of materials processing  and  OLED  design,  which  is  likely  to  be  found  in  scientific  literature  and  academic publishing (as opposed to grey literature).

## Thus, the aim of this review is to:

- o Review all recent peer-reviewed papers examining OLED devices using a solution-processed and TADF EML;
- o Examine  the  concepts  of  TADF  and  solution  processing  in  organic  semiconductors,  and identify any issues uniquely associated with OLED devices employing both phenomena, incl. synergistic effects; and
- o Highlight significant findings and identify a direction for future studies regarding solution processability, TADF and economic design of OLEDs.

Given the relatively low number of studies with exact relevance (i.e. development or discussion of OLED devices with both SP and TADF), articles are reviewed on a case-by-case basis and categorised with similar papers. Then, the findings are summarised and discussed with respect to the aims listed above. Articles not showing significant findings or discussions relevant to the advancement of SP TADF OLEDs or low-cost processing are not discussed here. Whereas other recent reviews on SP TADF OLEDs focus on novel molecular designs and structure-property relationships [19,20], this review retains focus on factors that contribute towards low cost manufacturing and the ability to be translated from research to commercialisation.

Table 1. Performance factors of solution processed, thermally activated delayed fluorescence OLEDs found in recent literature

| Reference   | Photoluminescence Quantum Yield (PLQY) (%)   | Photoluminescence Quantum Yield (PLQY) (%)   | Singlet- Triplet Splitting ∆E ST   | Photolumiscence Wavelength, λ PL (nm)   | Photolumiscence Wavelength, λ PL (nm)   | Maximum External Quantum Efficiency (EQE max )   |
|-------------|----------------------------------------------|----------------------------------------------|------------------------------------|-----------------------------------------|-----------------------------------------|--------------------------------------------------|
|             | Solution                                     | Film                                         | (eV) a                             | Solution                                | Film                                    | (%)                                              |
| [21]        | 26                                           | 26                                           | 0.1                                | 550                                     | 540                                     | 9.3                                              |
| [22]        | 94                                           | 52                                           | 0.03                               |                                         |                                         | 2.4                                              |
| [22]        | 100                                          | 31                                           | 0.06                               |                                         |                                         | 3.4                                              |
| [22]        | 94                                           | 8.5                                          | 0.06                               |                                         |                                         | 1.5                                              |
| [23]        | 92                                           | 52                                           | 0.13                               |                                         |                                         | 6.0                                              |
| [23]        | 95                                           | 40                                           | 0.07                               |                                         |                                         | 9.4                                              |
| [23]        | 96                                           | 45                                           | 0.08                               |                                         |                                         | 9.5                                              |
| [23]        | 95                                           | 49                                           | 0.07                               |                                         |                                         | 8.2                                              |
| [24]        | 76                                           |                                              | 0.07                               |                                         |                                         | 16.1                                             |
| [24]        | 70                                           |                                              | 0.09                               |                                         |                                         | 16.0                                             |
| [25]        | 34                                           |                                              | 0.058                              | 575                                     |                                         | 17.5                                             |
| [25]        | 37                                           |                                              | 0.048                              | 608                                     |                                         | 15.2                                             |
| [26]        | 11                                           | 12                                           | 0.12                               | 478                                     |                                         | 1.0                                              |
| [26]        | 20                                           | 47                                           | 0.05                               | 484                                     |                                         | 8.9                                              |
| [26]        | 65                                           | 95                                           | 0.01                               | 509                                     |                                         | 13.9                                             |
| [27]        | 55                                           |                                              | 0.07                               | 536                                     | 560                                     |                                                  |
| [27]        | 16                                           |                                              | 0.31                               | 429                                     | 424                                     |                                                  |
| [16]        | 94                                           |                                              |                                    |                                         |                                         | 8.1                                              |
| [16]        | 67                                           |                                              |                                    |                                         |                                         | 8.2                                              |
| [16]        | 78                                           |                                              |                                    |                                         |                                         | 18.1                                             |
| [28]        | 45                                           |                                              | 0.18                               |                                         |                                         |                                                  |
| [28]        | 98                                           |                                              | 0.13                               |                                         |                                         |                                                  |
| [29]        |                                              |                                              |                                    |                                         |                                         | 4.43                                             |
| [30]        |                                              |                                              |                                    |                                         |                                         | 12.9                                             |
| [30]        |                                              |                                              |                                    |                                         |                                         | 12.4                                             |
| [24]        | 44                                           |                                              | 0.07                               |                                         |                                         |                                                  |
| [31]        |                                              |                                              |                                    |                                         |                                         | 7.0                                              |
| [31]        | 68                                           |                                              | 0.09                               | 498                                     | 492                                     | 12.2                                             |
| [31]        | 48                                           |                                              | 0.20                               | 484                                     | 464                                     | 2.2                                              |
| [32]        |                                              |                                              |                                    |                                         |                                         | 9.4                                              |
| [32]        |                                              |                                              |                                    |                                         |                                         | 9.9                                              |

|         |     |     |      |     |     | 15    |
|---------|-----|-----|------|-----|-----|-------|
|         |     |     |      |     |     | 16    |
| [26]    | 11  |     | 0.12 | 478 |     | 1.0   |
|         | 20  |     | 0.05 | 484 |     | 8.9   |
|         | 65  |     | 0.01 | 509 |     | 13.9  |
| [33]    |     |     |      | 478 |     | 1.2   |
|         |     |     |      | 492 |     | 1.1   |
|         |     |     |      | 498 |     | 4.0   |
|         |     |     |      | 506 |     | 4.3   |
| [34]    | 71  |     | 0.16 |     |     | 18.7  |
| [35]    |     |     |      |     |     | ~24   |
| [36]    |     |     |      |     |     | 2.3   |
|         |     |     |      |     |     | 11.05 |
| [37]    | 44  |     | 0.18 | 590 | 553 | 1.2   |
|         | 56  |     | 0.17 | 594 | 545 | 5.5   |
|         | 71  |     | 0.20 | 591 | 541 | 11.8  |
| [38]    | 42  |     | 0.24 |     |     | 1.56  |
|         | 61  |     | 0.23 | 490 | 460 | 12.6  |
| [39]    | 46  | 75  | 0.21 | 510 | 477 | 2.4   |
|         | 2   | 39  | 0.05 | 608 | 522 | 3.7   |
| [40]    |     |     | 0.24 | 439 | 445 | 23.8  |
|         | 78  |     | 0.22 | 452 | 475 | 23.5  |
| [41]    | 12  |     | 0.04 |     | 549 | 8.1   |
| [42]    |     | 28  | 0.11 |     | 572 | 5.8   |
|         |     | 52  | 0.05 |     | 612 | 7.5   |
| [43]    |     |     |      |     |     |       |
| [44]    | 3.8 | 25  | 0.15 | 407 | 473 |       |
|         | 65  | 65  | 0.08 | 483 | 505 | 4.3   |
| [45,46] |     | 92  | 0.13 | 510 | 507 | 14.9  |
| [47]    | 76  | 74  | 0.06 | 443 |     | 17.8  |
|         | 81  | 1.0 | 0.06 | 453 |     | 20.0  |
| [48]    | 77  |     | 0.11 | 520 |     | 12.0  |
|         | 75  |     | 0.15 | 499 |     | 5.2   |
| [49]    | 74  |     | 0.04 | 606 |     | 9.0   |
| [50]    | 32  |     | 0.28 | 502 |     | 1.09  |
|         | 58  |     | 0.20 | 490 |     | 6.5   |
|         | 76  |     | 0.20 | 487 |     | 10.1  |
| [51]    | 60  | 42  | 0.33 | 421 |     |       |
|         | 64  | 58  | 0.25 | 438 |     |       |

|      | 52   | 22          | 0.17   | 451   |      |
|------|------|-------------|--------|-------|------|
| [52] |      |             |        |       | 5.7  |
|      |      |             |        |       | 3.6  |
| [53] |      | 63          |        | 444   | 1.4  |
|      |      | 71          |        | 444   | 2.0  |
|      |      | 64          |        | 448   | 1.2  |
| [54] |      | 0.8         | 0.1    | 550   | 13.9 |
| [55] | 2.1  | 56 (powder) | 0.18   | 590   | 3.18 |
|      | 45   | 87 (powder) | 0.17   | 536   | 3.72 |
|      | 30   | 75 (powder) | 0.18   | 540   | 8.47 |
| [56] | 61   |             | 0.06   | 465   | 19.1 |
|      | 94   |             | 0.05   | 476   | 8.0  |
| [57] | 88   | 52          | 0.17   |       | 15.5 |
|      |      |             |        |       | 17.1 |
| [58] |      | 44          | 0.2    | 550   | 10.0 |
| [59] |      |             | 0.35   | 533   | 20.1 |
|      |      |             | 0.46   | 536   | 15.2 |
|      |      |             | 0.42   | 539   | 1.8  |
|      |      |             | 0.40   | 556   | 1.4  |
| [60] | 50   | 39          |        | 507   |      |
|      | 67   | 74          |        | 511   | 16.1 |
|      | 66   | 70          |        | 512   |      |
|      | 60   | 59          |        | 513   |      |

- Calculated via the singlet (S1) and triplet (T1) energies determined via onset of fluorescence and
- a phosphorescence.

Table 1 presents a comparison of literature on OLED devices employing both SP and TADF within the emissive layer. To maintain concision, only primary performance figures are included to allow for general comparison of device performances across studies. Photoluminescence quantum yield, or  PLQY  (%),  describes  the  ratio  of  photons  emitted  to  photons  absorbed  during  controlled photoluminescence  in  either  solution  or  neat  film  states.  Singlet-triplet  splitting,  or ∆ EST (eV), represents the energetic difference between the lowest singlet (S1) and triplet (T1) electronic states, which  can  be  conceptualised  as  the  energetic  gap  electrons  must  overcome  through  Reverse Intersystem Crossing (RISC) and emit via the delayed fluorescence pathway. Photoluminescence wavelength, or λ PL (nm), describes the wavelength of emission during photoluminescence in the solution or neat film states, which is indicative of colour. External Quantum Efficiency, or EQE (%), describes the ratio of photons emitted to electrons injected during controlled electroluminescence, which reflects the overall device efficiency.

Detailed analyses and discussions of each study are included in the following sections.

## Polymers

The foremost benefit of polymers is their high solubility in organic solvents due to their long aliphatic chains. On the other hand, their large size and variability in molecular structure between production batches  results  in  difficulties  controlling  molecular  design  factors  that  affect  TADF  emission performance. An example of such a design factor is the distances and torsions between donor and acceptor moieties; both must be separated in order to reduce overlap of the HOMO and LUMO (typically localised around the donor and acceptor, respectively), which is directly related to ∆ EST [61].

In 2015, Nikolaenko, et al. [58] developed an SP TADF Emissive Layer (EML) made of a polymeric material. In this case, the donor and acceptor moieties served as distinct monomers in the greater polymer chain, and polymerisation amounts were controlled to vary charge transport properties and  buffer  the  recombination  zone.  Other  monomers  were  selectively  added  to  control  the electronic, optical and physico-chemical properties, such as solubility and viscosity, and a blockpolymer  structure  was  used  to  ensure  tight  control  of  polymer  sequence.  Interestingly,  the experimental values of the containing devices showed a relatively low PLQY (in air) of 41% with estimated RISC yields of 83%, suggesting that light conversion, rather than triplet conversion, was limiting the efficiency of the device. Finally, the authors noted that the long-chain nature of the polymer EML may have resulted in horizontal alignment of the dipole moment of the EML polymer with the substrate, which is known to improve efficiency [62,63].

Nobuyasu,  et  al.  [36]  continued  the  foray  into  TADF  polymers.  Devices  were  made  using  two copolymers consisting of a known small molecule emitter. Both solution-processed polymer devices showed  significantly  lower  efficiencies  than  vacuum-deposited  small  molecule  devices  and exhibited noticeable roll-off. Regardless, the authors noted that their polymer device efficiencies were comparable to those of the major polymer TADF effort by Nikolaenko, et al [58] the previous year.  The  low  polymer  performance was attributed to weak electronic properties as a result of unrefined  solution-processing  methods,  without  any  further  discussion  given.  The  authors presented two primary challenges of TADF polymers: i) high molecular weight compounds cause high ∆ EST and non-radiative internal conversion, effectively reducing the efficiency; and ii) TripletTriplet Annihilation (TTA) is frequent in polymers, creating an alternative non-radiative pathway for triplet  excitons  besides  RISC.  While  the  solubility  of  polymers  makes  them  attractive  for  OLED devices, these issues need to be rectified before seeing commercial use.

Zhu, et al. [46] developed a conjugated polymer for use in a SP TADF OLED. In contrast to the typical alternating D-A backbone structure seen in most emissive polymers, acceptors were perpendicularly grafted to a backbone of donors to increase torsion, thus increasing HOMO-LUMO separation and reducing ∆ EST.  Despite  the  unique  electronic  and  optical  properties  of  conjugated  polymers  for optoelectronics [64,65],  the  characteristic effects of conjugated  polymers  on  the  current  device were not discussed.

The same polymer was used in an SP TADF OLED by Lin, et al. [45]. They observed high rates of triplet exciton quenching and attributed it to intra- and inter-molecular accumulation quenching between polymer chains. This accumulation quenching in TADF, which was recently studied, occurs via the close-range, electron-exchange Dexter energy transfer mechanism, as opposed to the long-range, dipole-dipole Forster mechanism [66]. To circumvent the accumulation quenching, they added an interfacial exciplex host to improve RISC rates and bolster the delayed fluorescence contribution. Indeed, quenching and roll-off were significantly reduced as evidenced by L50 and J50 (i.e. luminance and current density after EQE has reduced to 50% of maximum over prolonged operation), which were each increased nearly three-fold as compared to the pure polymer OLED.

A study by Xie, et al. [60] developed an SP TADF polymer using the same side-chain grafting strategy mentioned above and a TADF small molecule reported earlier [67,68] as an emissive repeating unit. The  devices  utilised  a  novel  transfer  mechanism  where  an  additional  TADF  small  molecule  was included  as  an  'assistant  dopant',  which  mediates  charge  transfer  between  the  host  and  TADF dopant and contributes towards a portion of the RISC processing of singlet excitons. Devices with optimised structure showed remarkable EQE of 16% with near 100% IQE. While the assistant dopant strategy is likely to improve device efficiencies, a three-component-EML is likely to require extra design considerations and, consequently, production costs for commercial production. Interestingly, the results also indicated that RISC rates are higher in polymers than small molecules.

Ren, et al. [59] developed a series of copolymer and homopolymer SP TADF OLEDs to illustrate the effects  of  polymer  structure  on  TADF  performance.  In  this  case,  emissive  pendant  moieties consisting of a phenothiazine donor and dibenzothiophene-dioxide acceptor were partitioned by inert styrene moieties in the greater polymer chain. This design was intended to boost emissive efficiency by reducing intermolecular interactions between pendant units. Indeed, the copolymers showed much lower ∆ EST and significantly higher EQE, Current Efficiency (CE) and Power Efficiency (PE) than the homopolymer, and copolymers showed increasing performance along with increasing degree of copolymerisation (i.e. ratio of styrene units to emissive units). Partitioning the emissive units  was  believed  to  reduce  quenching  via  internal  conversion  and  triplet-triplet  annihilation. However, no discussion was provided on the effect of molecular structure on solubility.

## Small Molecules

Small molecules are relatively low molecular weight (as compared to polymers) tightly-packaged molecules that form discrete particular neat films. As opposed to polymers, small molecules are not always soluble in ideal solvents, and thus present an extra complication if solution processing is desired. On the other hand, the tightly-packed, discrete particle film structure of small molecular neat films are more electrically conductive and thermally stable than polymers, and are thus more resistant to dissociation after formation of the neat film. A review of solution-processable small molecules for OLEDs can be found here [15].

In what might be the first of its kind, Cho, et al. [16] produced three separate solution processed TADF devices with EQEmax values of up to 18.1%. One emitter - t4CzIPN - showed higher device efficiencies when fabricated via solution processing instead of vacuum deposition. In this case, it was believed that the t-butyl moiety improved solubility (0.4%) as compared to other designed emitters (0.1%) and resulted in a more stable film morphology. Further discussion purported that greater solubility resulted in a more uniform distribution in the final film which: i) subdues exciton quenching; and ii) minimises interstitials and defects, which lead to charge trapping - both of these factors  will  reduce  overall  quantum  efficiency.  Furthermore,  when  deposited  in  higher  doping concentrations (3% and 5%), the resultant film morphology was noticeably more disrupted, which was believed to cause more charge trapping. Indeed, these devices showed lower current densities and quantum efficiencies. As noted earlier, the higher solubility of the t4CzIPN emitter might well be a result of the longer and more planar carbon backbone.

Cho et al. [47] developed highly efficient solution processed TADF emitters by modifying 4CzIPN, replacing either 1 or 2 CN groups with F atoms (3CzFCN and 4CzFCN). The rationale behind the design was to use the hydrophobic nature of F to counteract the hydrophilicity of CN and improve solubility in organic solvents. Indeed, the novel molecules showed higher solubility in toluene, and the solubility increased according to number of F moieties (1.5 wt% for 3CzFCN, 1.0 wt% for 4CzFCN and 0.1 wt% for 4CzIPN [69]). It is important to note that toluene is commonly required for TADF studies for its ability to prevent PL quenching of TADF molecules in solution. AFM revealed a much

greater film morphology in 3CzFCN as a result of its higher dissolution in toluene. Furthermore, it was also believed that the weak electron withdrawing nature of the F moiety, relative to the parting CN, caused a slight bathochromic shift in the PL emission (443 nm and 453 nm for 3CzFPN and 4CzFPN, respectively, from 470 nm of 4CzIPN [69]). The study indicates that while functionalisation may be a simple yet effective method to improve solubility, PL or electrodynamic characteristics are likely  to  change  -  this  might  be  particularly  more  pronounced  in  TADF  molecules  due  to  their delicate electronic nature.

The same group [34] later tried to improve the unstable emissive lifetimes of their previous efforts through a benzonitrile core substituted with 5 carbazole units (5CzCN). The aim of the design was to increase solubility by agglomerating as many donors as possible (while retaining the CN unit) in order to increase both the donor-acceptor dihedral torsion and the available surface area for solvent penetration. Indeed, the additional carbazole increased solubility in toluene from 0.1% for 4CzIPN, as per their previous study [69], to 0.5% for 5CzCN. However, it should be noted this figure is lower than the fluorinated benzonitriles of the group's previous effort mentioned above. Furthermore, while the lifetime was aimed to improve through extending conjugation of the benzonitrile acceptor and increase aromatic units through carbazole functionalisation, notable lifetime improvements were only detected in vacuum-deposited devices.

Kim, et  al.  [35]  focused  on  improving  production  costs  not  only  through  soluble  molecules,  but through simplifying device structures. The aim was to create a device with no transport layers by using a 'self-organised buffer hole injection layer' (Buf-HIL). 4CzIPN dopant and CBP host were used as  the  EML.  The  Buf-HIL  consisted  of  PEDOT:PSS  and  a  perfluoric  acid  copolymer  (PFI),  which resulted in a neat film with graded PFI concentration - the lower surface energy of PFI allows for natural  self-organisation  during  spin  coating.  This  gradient  caused  the  work  function  to  change across the Buf-HIL, allowing each end to closely match the electronic levels of its neighbouring layer and  improve  internal  hole  transport  and  reduce  hole  accumulation  at  the  interface  (i.e.  work function of the bottom end was similar to the anode, and that of the top matched with the HOMO of the host material). Additionally, the Buf-HIL also improved efficiency by reducing contact between excitons and the lower energy levels of PEDOT:PSS, which has been reported to result in exciton quenching [70,71]. A polar aprotic solvent, THF, was selected to dissolve the highly polar 4CzIPN indeed, solubilities were much higher in THF (&gt;10%) than in toluene (&lt;1%). THF not only improved film uniformity, it significantly reduced aggregation of 4CzIPN, resulting in a two-fold increase in PL intensity from a film spun from toluene as a result of aggregation-caused quenching. The authors found that solvents with higher dipole moments resulted in greater morphology and PL intensity. Ultimately, the study demonstrates a resourceful method to simultaneously improve both device efficiency and manufacturability.

Adachi's group [70] performed a comparative study of a series of 4CzIPN devices with either CBP or CPCB  host,  solution  or  vacuum  processed  layers  and  varying  Electron  Transport  Layers  (ETL). Interestingly,  CBP  devices  showed  no  notable  variation  in  EQEmax  between  solution  or  vacuum processed devices, while those of CPCB showed up to a 31% decrease. Lifetimes were significantly lower in most devices when solution processed. However, solution processed CPCB devices had much improved lifetimes than solution processed CBP devices, which was attributed to a higher molecular weight, greater solubility and better film morphology.

Xie  et  al.  [25]  developed  two  small-molecule  emitters  that  were  both  vacuum  and  solution deposited and compared. The solution deposited devices of each molecule showed comparable EQEs to their vacuum-deposited counterparts - this was even more notable considering that the vacuum deposited devices did not include hole transport layers.

Not long after the worldwide recognition of TADF, Chen, et al. [55] developed one of the first and most notable devices utilising both TADF and solution processability. The idea was to utilise the inherent narrow ∆ EST found in transition metal complexes for TADF without the natural instability of  rare  phosphorescent  transition  metals  like  iridium  or  platinum.  The  same  group  [28]  later developed  a  cuprous-complex  small  molecule  which  showed  clear  TADF  in  solution  processed devices. The device was made by using a carbazole-based molecule, czpzpy, as both a ligand and host material for a separate emissive dopant, [Cu(CH3CN)2(POP)]BF4    - both materials were simply spin deposited in tandem without prior preparation. The ligand was used in excess as an attempt to reduce dissociation of the emissive dopant and thus improve PLQY in the device.

Verma, et al. [54] developed a copper iodide complex for use in an inkjet-printed EML. A CopperIodide core was substituted with alkyl phosphites to improve solubility in nonpolar solvents suitable for  inkjet  deposition.  The  molecular  design  rationale  was  to  include  asymmetrically-substituted ligands  in  order  to  reduce  the  conformational  possibilities,  thereby  increasing  the  entropy contribution and solubility. Solubilities in polar solvents such as ethanol were between 10 - 30 mg mL -1 but were higher than 100 mg mL -1 for non-polar solvents. The devices with a printed EML and evaporated organic layers showed an EQEmax of 13.9%. With the broad solubility behaviour, the authors noted that the molecule was suitable for various types of high-perfomance inks and print heads - the molecule could be dissolved in solvents with tuneable viscosity or surface interactive behaviour.

Sun,  et  al.  [53]  developed  solution  processed  TADF  EMLs  with  thermally  crosslinkable  host  and dopant. The desire for crosslinking EML materials was not made completely clear, but it was believed to contribute to a greater thermal stability and more homogenous film morphology. The device with a film of host:dopant mass ratio of 1:0.09 showed the best performance compared to those of 1:0.06 and 1:0.12, but the reason was not elaborated on.

Chen, et al. [56] developed a solution processed, non-doped, TADF emitter showing an EQEmax of 19.1% - reportedly the highest as at publication (Oct 2017). This breakthrough was attributed to a dual-charge-transfer mechanism, in which charge was transferred both through conventional D-A transport as well as through-space electron transfer in this case, electrons from the π -orbitals of donor and acceptor moieties in close proximity transfer through space [72,73]. Having an alternate pathway for charge transfer was believed to result in higher dipole moment and lower ∆ EST.

Huang, et al. [43] developed a TADF molecule with mechanochromic luminescence - colour variation depending on the solution with which the molecule was deposited. The molecule, Cz-AQ, emitted as a deep red at 680 nm when deposited through dichloroethane and yellow at 600 nm through a mixture of dichloroethane and ethanol (equivalent volume ratio). Crystals of the molecule were grown  through  different  solutions  and  the  crystallographies  were  studied  to  examine  the luminescent behaviour. Between the two crystals, one showed stacking with an H-type aggregation along with b axis, leading to strong π π interactions induced by -significant orbital superimposition this was believed to cause the red shift in emission of the deposited films. TGA and DSC also revealed transition of emission colour from red to yellow in the same crystal after thermal decomposition. Unfortunately, the specific solvatochromic effect on the molecule (i.e. the mechanism by which different solvents affect the molecular orientation and emission wavelength) was not discussed. It is also  worth  noting  that  due  to  the  closely  stacked  molecular  orientation,  Cz-AQ  showed aggregation-induced emission (AIE) properties - a mechanism in which luminescence is enhanced in aggregated states such as neat films [74].

Dendrimers serve as a new class of molecules with sizes in between those of small molecules and polymers.  Dendrimers  are  identified  by  their  tree-like structure, with 'branch'  molecules surrounding a single core in three dimensions. These branches then attach to subsequent branch molecules,  thus  giving  the  dendrimer  a  tree-like  structure.  Branch  molecules  are  referred  to  as dendrons, while the number of branches in succession is termed 'generation'. Dendrimers are often designed using some existing small molecule as either dendrons or the core molecule. A typically high  molecular  weight  ensures  a  good  degree  of solubility  in  common  solvents,  but  also  avoids forming inhomogeneous, impure or poorly distributed thin films that often occur in polymers with indefinite  molecular  weight  [15].  While  review  articles  of  emissive  dendrimers  do  exist  [75,76], functional dendrimer OLED devices have only appeared in the literature within the last decade, and no relevant review articles have appeared since.

Albrecht, et al. [22] developed the first solution processable TADF OLED using a dendrimer-based emissive  layer.  The  emissive  dendrimers  consisted  of  a  triazine  core  unit  attached  to  various generations  of  carbazole  dendrons  (up  to  4  generations).  Perhaps  since  Adachi's  novel  4CzIPN molecule [1], Carbazole has become well-known moiety for functionalising TADF molecules because of its hole-transport velocity, high triplet energy, stable thermal resistance and its ability to improve solubility  and  resultant  film  morphology  [31,77].  It  was  found  that  higher  generation  number resulted in worse performance in regard to ∆ EST and PLQY (film and solution), but the highest EQE came  from  3  generations.  The  increased  intermolecular  interactions  resulting  from  higher generation numbers was believed to be the cause of lower PLQY.    Regardless, each dendrimer showed clear TADF, indicating that dendrimers may well be the ideal solution to achieving both TADF and solution processability in future molecular designs. The authors also noted that carbazolebased  dendrimers  have  been  previously  shown  to  become  insoluble  after  photo-induced crosslinking  [78]  -  this  is  hugely  beneficial  for  solution  processed  devices,  as  it  will  allow  the deposited EML to remain solid after contact with solution of neighbouring layers.

This  orthogonal  dendrimer  and  a  device  with  fully  solution-processed  organic  layers  was  later developed by the same group through the use of a similar triazine- and carbazole-based dendrimer [23]. Part of the strategy was to include terminating functional groups on the final generation of carbazole dendrons to increase initial solubility. Terminating groups included methyl, t-butyl, phenyl and  dibenzocarbazole  substituents.  As  expected,  all  funtionalised  dendrimers  showed  good solubility  in  common solvents, such as chloroform, THF and toluene, and the dibenzocarbazolefunctionalised  dendrimer dissolved in hexane. However, no quantitative analysis nor qualitative speculation on the degree and change of solubility among variants was given. It was also shown that the functionalised dendrimers showed much better lifetimes than the non-functionalised - this was attributed to the electrochemical stability induced by the terminating groups, and the belief that the  non-functionalised  dendrimer might undergo electro-polymerisation in the powered device, which generated carrier traps.

The  same  group  then  continued  their  work  and  developed  devices  with  t-butyl-substituted dendrimer as a dopant and a carbazole-dendrimer-based hosts [24]. The motivation was to select a host that could improve the PLQY of previously developed devices while maintaining orthogonality or resistance to dissolution in alcohol used to deposit ETLs. Hosts with generation numbers higher than 2 showed near-complete resistance to alcohol (likely due to higher molecular weight [79]), while that of 2 nd generation was largely dissolved. Furthermore, a separate control experiment that even if the host is sufficiently resistant, alcohol can permeate the solid film of a host:dopant complex and dissolve the dopant, even if the dopant is intrinsically resistant to alcohol.

The most recent effort of Albrecht's group [52] involved a imparting AIE to a solution processable TADF dendrimer. Indeed, AIE was only noticed in dendrimers, as opposed to small molecules of similar composition, due to the intermolecular interactions occurring in dendritic structures - these

interactions inhibit intramolecular rotations and vibrations, which create non-radiative pathways. As noted in previous studies, the dendrimers showed good resistance to alcohols, which allows for solution deposition of neighbouring ETLs in alcohol without degradation of the EML. While the EQEs of these dendrimers were comparatively lower than the authors' previous work, the synergy of AIE with TADF and solution processability serves as an innovative method to improve both performance and cost effectiveness of devices. Hu, et al. [39] and Huang, et al. [42] recently reported molecules with AIE, TADF and solution processability, albeit with much less notable results.

Li  et  al.  [48]  developed  a  new  molecule  by  dendronising  a  DMAC-DPS  core  with  up  to  two generations  of t-butyl-substituted carbazole. Both  dendrimers  exhibited good  solubility in dichloromethane,  tetrahydrofuran,  toluene  and  chlorobenzene,  likely  boosted  by  the  t-butyl groups, but no quantitative solubility analysis was performed. High decomposition temperatures (471 o C  and  507 C  for  1  generation  and  2  generations,  respectively)  and  post-annealing  AFM o revealed very high thermal stability and morphological homogeneity after spin coating for both dendrimers. However, different devices showed minor changes in efficiency according to varying annealing temperatures - EQEs for the 1-generation-dendrimer device showed fluctuations up to nearly  4  percentage  points  through  annealing  at  25 C  to  160 C.  Regardless,  all  devices  showed o o relatively low roll-offs.

Ban, et al. [50] designed a dendrimer TADF emitter using alkyl, instead of π -conjugated or aromatic, chains to link dendrons to the emissive core. The rationale of this design was threefold: i) to improve solubility and film morphology by reducing molecular rigidity and steric hindrance; ii) to improve charge transport through non-conjugated linkers; and iii) to reduce emission quenching by using non-conjugated spacers to isolate the emissive core [80]. While the improvement to solubility and morphology  was  not  verified,  the  alkyl-linked  dendrimers  indeed  showed  improved  device performance, which was attributed to the effects predicted above. Electronic properties between dendrimers  showed  little  variance  (for  example,  relative  standard  deviation  of ∆ EST  between dendrimers was only 13%) - this is interesting to note as steric hindrance and rigidity are known to be greatly influential on electronic states in TADF molecules. Thus, aliphatic linkers may well be one method  to  reconcile  solution  processability  and  TADF.  The  same  group  later  witnessed  similar effects through yellow- [37] and blue-emitting [38] dendrimers.

Ban et al. [57] later developed the first TADF OLED using fully solution processable organic layers. The dendrimer emitter, a cyanobenzene with two generations of carbazole dendrons (Cz-CzCN), was used as a non-doped (self-host) EML. The high molecular weight dendrimer was designed to provide resistance to alcohol solvents in order to avoid orthogonal dissolution when depositing the ETL. Thus, neat films of Cz-CzCN and a single-generation molecule (5CzCN) were subjected to absorption spectroscopy  before  and  after  rinsing  in  isopropyl  alcohol  -  as  expected,  5CzCN's  absorption intensity reduced drastically, while that of Cz-CzCN only reduced by around 5%. Unfortunately, the mechanism behind the dendrimer's high alcohol resistance was not expounded on beyond the high molecular weight. Alkyl chains were used to link the 2 nd generation dendrons, which were believed to  enhance  overall  solubility  and  help  maintain  the  electronic  properties  of  the  emissive  core separate from dendrons. Furthermore, the encapsulating structure of dendrons was believed to limit exciton quenching via intermolecular interactions in the emissive core. Soon after, the same group [40] reported a new OLED device using similarly designed molecules (with 3 and 4 dendrons per generation instead of 5) as a host and guest EML, respectively. These devices were believed to use  the  same  phenomena  (i.e.  inhibition  of  exciton  quenching  via  molecular  encapsulation  and enhanced solubility via alkyl chain linkers) to achieve higher EQEs than the previous effort (EQEmax of  23.8%  and  23.5%  for  3  dendrons  and  4  dendrons,  respectively).  It  should  be  noted  that  this appears to be the highest EQE reported for a solution processed TADF device to date.

## Summary

## Synergistic effects

There do not appear to be any beneficial synergistic effects between TADF and SP; in other words, the effects of TADF and SP do not combine to boost performance to levels unexpected by each factor individually.  There  are,  however,  notable  detrimental  effects  -  soluble  materials  have  inherent properties that can affect the performance of TADFs and thus must be considered during design stages (and vice versa):

- o Deposition via solvent alters atomistic morphology and molecular orientation (as compared to solid crystalline structure), and  thus effects the electron orbital configuration. Consequently, this has significant effects on the excitonic and electronic pathways, which will alter photo- and electroluminescent efficiencies;
- o Different types of solvents will alter emission characteristics, whether through alterations to the film structure, molecular orientation or both;
- o Both  TADF  contribution  and  solubility  are  currently  precisely  controlled  by  molecular structure - altering structure to tune one property is likely to affect the other. For example, increasing  alkyl  chain  length  to  increase  solubility  may  separate  donor  and  acceptor moieties, disrupting the charge transfer mechanism or ∆ EST; and
- o Solution processed neat films are expected to have greater decay lifetimes [70]. This may disrupt the contributions to fluorescence from different sources (i.e. delayed or prompt).

It  appears  any  breakthroughs in SP-TADF OLEDs will occur through trial and error and empirical observations of new molecular designs (as opposed to mechanistic analysis).

## Molecular Type

Polymers have higher solubilities as a result of the longer aliphatic chain. However, the electronic performance of TADF polymers is initially at a disadvantage as the length, complexity and variability of polymer structures introduces difficulties in tuning the structure-related properties of TADF (e.g. ∆ EST and consequent IQE, which are related to D-A separation). On the other hand, small molecules are  smaller  and  more  precise  in  nature,  allowing  one  to  tune  structure-related  properties  and performances through minor alterations to molecular structure or composition. Furthermore, they are also associated with simpler and more controllable synthesis methods, which is likely to reduce the costs of large-scale production. Finally, assuming a decent dissolution, small molecules generally produce well-ordered,  neatly-packed  thin  films,  resulting  in  greater  electronic  performance  and lifetime.

Dendrimers are a great middle ground for low-cost design, capturing the solubility of polymers with the  facile  synthesis  methods  and  the  ability  to  precisely  control  molecular  structure  of  small molecules.  Dendrimers  are  suitable  for  TADF  emission  as  the  electronic  structure  and  exciton transmission can be tuned through addition and modification of dendrons. Additionally, molecular weight can be largely varied by tuning the number and structure of dendrons; this allows one to selectively  tune  solubility  and/or  resistance  to  orthogonal  solvents.  Ken  Albrecht's  group  has performed a number of studies into the characteristics of dendrimers and development of suitable dendrimer-based  SP  TADF  OLEDs.    Future  work  could  focus  on  finding  novel  dendrimer  and dendron structures for optimal performance along with suitable solvents and device structures.

## Future Research

## Solubility

While  recognised  as  a  critical  factor  for  OLED  design,  few  experimental  studies  actually  discuss solubility or the consideration thereof before design. Since solubility is not easily quantified, many researchers simply rely on qualitative descriptors such as length of alkyl chains or molecular size to evaluate solubility. Glass transition temperature is one parameter that is associated with solubility [15,81].  While  many  of  the  studies  reviewed  herein  do  determine  Tg  as  part  of  experimental procedure, none have discussed it with regards to solubility. Instead, more effort should be given to quantify  solubility  and  develop  generic  correlations  between  solubility  and  device  stability  or performance. In a review on SP small molecules for OLEDs, Duan, et al. [15] noted that the effect of solvent on solubility and film quality needs further investigation. The Solubility Parameter [82,83] attempts to numerically predict interactive dissolution via the intermolecular and diffusive forces. Derivations of the solubility parameter method have been used to study ink-based deposition of organic  semiconductors  in  some  theoretical  studies  [84-87],  albeit  with  unpredictable  results. Sanders,  et  al.  [88]  recently  developed  a  methodical  design  process  for  OLED  materials  determination of solubility parameters through computational molecular dynamics (MD) simulations was included in one step. Numerical correlations between solubility and resultant film properties would assist future researchers in SP OLED design.

## SP-electrodes

While solution processability is important in organic emissive materials, each device layer, including the electrode material, must be compatible with R2R processes in order to experience complete low-cost, large-scale manufacturing; this includes the electrode, which is typically metallic. Several articles have been devoted to SP metallic electrodes via deposition of metallic ink - a suspension of metallic nanoparticles in a colloidal system [89-93]. Unfortunately, as is common in bulk electrodes, this research focuses on the noble metals Au or Ag, which are not economically suitable for largescale manufacture. As an alternative, Lee, et al. [94,95] have studied Al-based electrodes deposited via  metallic  ink  and  roll-to-roll  process,  and  have  recently  reported  a  functional  touch-sensitive panel with apparent resistance to oxidation. Cu, with its high inherent conductivity, may be another suitable  candidate  -  as  discussed  earlier,  Cu-based  TADF  molecules  have  already  been  solution processed. Widespread attention is given to carbon nanotube- or graphene- based cathodes, which have given promising electrical performances and are easily adapted to wet-deposition [89,96,97]. Polymer cathodes may be a viable alternative as they have been studied for use in batteries [98-103] and, to a lesser extent, nanoscale batteries [104] and solar cells [105].

Designers should also consider the solution processability of organic transport layers for fully SP OLEDs. However, transport layers have fewer design criteria than EMLs, and will not experience the same number of detrimental synergistic effects when depositing via solution as discussed earlier. Thus, there are fewer considerations when incorporating SP transport layers. Solvent orthogonality is perhaps the most significant consideration.

## Inkjet Deposition

The majority of SP-OLED studies use spin coating as the chosen method for deposition. While spin coating is indeed a wet process and allows one to analyse film structure, it does not necessarily translate into large-scale manufacture. Not only is the physical process of spin coating not applicable to the large scale, it cannot be incorporated into R2R processes. On the other hand, inkjet deposition

is compatible and thus more suitable for commercial manufacture. In fact, electronic developers have recently begun using inkjet deposition in production lines or unveiled inkjet-deposited OLED prototypes. Thus, by using inkjet deposition in initial studies, researchers can ensure any developed materials are suitable for manufacture immediately and skip additional steps involved in translating their research to the market.

## Single-layer and non-doped devices

More efforts should be paid towards reducing production costs through single-layer devices and non-doped  (i.e.  no  host)  EMLs.  Not  only  will  this  minimise  production  costs  through  reducing materials consumption, it will lessen the number of factors needing to be considered during design stages, thus simplifying the overall design procedure. As an example, doped EMLs require additional consideration of the entire electronic structure of the dopant along with that of the host. Similarly, in a fully-solution processed device, each layer needs a high level of orthogonal resistance to certain solvents  to  avoid  dissolution  when  depositing  neighbouring  layers;  single-layer  devices  will  not require such consideration. In recent years, non-doped EMLs have made substantial progress in the literature, boasting greater stability and somewhat similar performance efficiency when compared to  their  doped  counterparts  [106].  On  the  other  hand,  single-layer  OLEDs  are  considerably  less common  in  research;  the  few  notable  recent  studies  of  single-layer  OLEDs  in  literature  show significantly lower performance efficiencies (for example, see [107,108]). Light emitting electrochemical cells, which operate by a slightly different mechanism, are a perfect example of solid-state lighting through minimalistic single-layer design [109]. The Zysman-Colman group [110113] have produced several light-emitting electrochemical cells using TADF EMLs, albeit at reduced efficiencies.

## Conflicts of interest

The author declares no conflicts of interest.

## References

- 1. Uoyama, H.; Goushi,  K.;  Shizu,  K.;  Nomura,  H.;  Adachi,  C.  Highly  efficient  organic  light-emitting diodes from delayed fluorescence. Nature 2012 , 492 , 234, doi:10.1038/nature11687

## https://www.nature.com/articles/nature11687#supplementary-information.

- 2. Parker,  C.A.;  Hatchard,  C.G.  Triplet-singlet  emission  in  fluid  solutions.  Phosphorescence  of  eosin. Transactions of the Faraday Society 1961 , 57 , 1894-1904, doi:10.1039/TF9615701894.
- 3. Kaji, H.; Suzuki, H.; Fukushima, T.; Shizu, K.; Suzuki, K.; Kubo, S.; Komino, T.; Oiwa, H.; Suzuki, F.; Wakamiya,  A.J.N.c.  Purely  organic  electroluminescent  material  realizing  100%  conversion  from electricity to light. 2015 , 6 , 8476.
- 4. Zhang, Q.; Tsang, D.; Kuwabara, H.; Hatae, Y.; Li, B.; Takahashi, T.; Lee, S.Y.; Yasuda, T.; Adachi, C.J.A.M. Nearly 100% internal quantum efficiency in undoped electroluminescent devices employing pure organic emitters. 2015 , 27 , 2096-2100.
- 5. Lin, T.A.; Chatterjee, T.; Tsai, W.L.; Lee, W.K.; Wu, M.J.; Jiao, M.; Pan, K.C.; Yi, C.L.; Chung, C.L.; Wong, K.T.J.A.M. Sky-blue organic light emitting diode with 37% external quantum efficiency using thermally activated delayed fluorescence from spiroacridine-triazine hybrid. 2016 , 28 , 6976-6983.
- 6. Moon, C.-K.; Suzuki, K.; Shizu, K.; Adachi, C.; Kaji, H.; Kim, J.-J. Combined Inter- and Intramolecular Charge-Transfer  Processes  for  Highly  Efficient  Fluorescent  Organic  Light-Emitting  Diodes  with Reduced Triplet Exciton Quenching. Advanced Materials 2017 , 29 , 1606448, doi:doi:10.1002/adma.201606448.
- 7. Yersin, H. Highly Efficient  OLEDs: Materials Based on Thermally Activated Delayed Fluorescence ;  Wiley: 2018.
- 8. Koden, M. OLED Displays and Lighting ; Wiley: 2016.
- 9. Volz,  D. Review  of  organic  light-emitting  diodes  with  thermally  activated  delayed  fluorescence  emitters  for energy-efficient sustainable light sources and displays ; SPIE: 2016; Vol. 6, pp. 13.
- 10. Im,  Y.;  Kim,  M.;  Cho,  Y.J.;  Seo,  J.-A.;  Yook,  K.S.;  Lee,  J.Y.  Molecular  Design  Strategy  of  Organic Thermally  Activated  Delayed  Fluorescence  Emitters. Chemistry  of  Materials 2017 , 29 , 1946-1963, doi:10.1021/acs.chemmater.6b05324.
- 11. Santos, P.L.; Ward, J.S.; Data, P.; Batsanov, A.S.; Bryce, M.R.; Dias, F.B.; Monkman, A.P.J.J.o.M.C.C. Engineering the singlet-triplet energy splitting in a TADF molecule. 2016 , 4 , 3815-3824.
- 12. Bergmann,  L.;  Zink,  D.M.;  Bräse,  S.;  Baumann,  T.;  Volz,  D.  Metal-Organic  and  Organic  TADFMaterials: Status, Challenges and Characterization. In Photoluminescent Materials and Electroluminescent Devices , Springer: 2017; pp. 201-239.
- 13. Yersin, H.; Czerwieniec, R.; Shafikov, M.Z.; Suleymanova, A.F.J.C. TADF  Material Design: Photophysical Background and Case Studies Focusing on CuI and AgI Complexes. 2017 , 18 , 3508-3535.
- 14. Dias,  F.B.;  Penfold,  T.J.;  Monkman,  A.P.  Photophysics  of  thermally  activated  delayed  fluorescence molecules. Methods and applications in fluorescence 2017 , 5 , 012001.
- 15. Duan, L.; Hou, L.; Lee, T.-W.; Qiao, J.; Zhang, D.; Dong, G.; Wang, L.; Qiu, Y. Solution processable small molecules for organic light-emitting diodes. Journal of Materials Chemistry 2010 , 20 , 6392-6407.
- 16. Cho, Y.J.; Yook, K.S.; Lee, J.Y. High Efficiency in a Solution-Processed Thermally Activated DelayedFluorescence  Device  Using  a  Delayed-Fluorescence  Emitting  Material  with  Improved  Solubility. Advanced Materials 2014 , 26 , 6642-6646, doi:doi:10.1002/adma.201402188.

- 17. Nie,  H.;  Hu,  K.;  Cai,  Y.;  Peng,  Q.;  Zhao,  Z.;  Hu,  R.;  Chen,  J.;  Su,  S.-J.;  Qin,  A.;  Tang,  B.Z. Tetraphenylfuran: aggregation-induced emission or aggregation-caused quenching? Materials Chemistry Frontiers 2017 , 1 , 1125-1129, doi:10.1039/C6QM00343E.
- 18. Jenekhe, S.A.; Osaheni, J.A. Excimers and Exciplexes of Conjugated Polymers. Science 1994 , 265 , 765768, doi:10.1126/science.265.5173.765.
- 19. Huang, T.; Jiang, W.; Duan, L. Recent progress in solution processable TADF materials for organic lightemitting diodes. Journal of Materials Chemistry C 2018 , 6 , 5577-5596, doi:10.1039/C8TC01139G.
- 20. Zou,  Y.;  Gong,  S.;  Xie,  G.;  Yang,  C.  Design  Strategy  for  Solution-Processable  Thermally  Activated Delayed Fluorescence Emitters and Their Applications in Organic Light-Emitting Diodes. Advanced Optical Materials 2018 , 6 , 1800568, doi:doi:10.1002/adom.201800568.
- 21. Lee, S.Y.; Yasuda, T.; Komiyama, H.; Lee, J.; Adachi, C. Thermally Activated Delayed Fluorescence Polymers for Efficient Solution-Processed Organic Light-Emitting Diodes. Advanced Materials 2016 , 28 , 4019-4024, doi:doi:10.1002/adma.201505026.
- 22. Albrecht, K.; Matsuoka, K.; Fujita, K.; Yamamoto, K. Carbazole Dendrimers as Solution-Processable Thermally Activated Delayed-Fluorescence Materials. Angewandte Chemie International Edition 2015 , 54 , 5677-5682, doi:doi:10.1002/anie.201500203.
- 23. Albrecht, K.; Matsuoka, K.; Yokoyama, D.; Sakai, Y.; Nakayama, A.; Fujita, K.; Yamamoto, K. Thermally activated delayed fluorescence OLEDs with fully solution processed organic layers exhibiting nearly 10% external quantum efficiency. Chemical Communications 2017 , 53 , 2439-2442, doi:10.1039/C6CC09275F.
- 24. Albrecht, K.; Matsuoka, K.; Fujita, K.; Yamamoto, K. A dendrimer emitter doped in a dendrimer host: efficient thermally activated delayed fluorescence OLEDs with fully-solution processed organic-layers. Materials Chemistry Frontiers 2018 , 2 , 1097-1103.
- 25. Xie, G.; Li, X.; Chen, D.; Wang, Z.; Cai, X.; Chen, D.; Li, Y.; Liu, K.; Cao, Y.; Su, S.-J. Evaporation- and Solution-Process-Feasible Highly Efficient Thianthrene9,9′,10,10′ -Tetraoxide-Based Thermally Activated Delayed Fluorescence Emitters with Reduced Efficiency Roll-Off. Advanced Materials 2016 , 28 , 181-187, doi:doi:10.1002/adma.201503225.
- 26. Liu,  Y.;  Xie,  G.;  Wu,  K.;  Luo,  Z.;  Zhou,  T.;  Zeng,  X.;  Yu,  J.;  Gong,  S.;  Yang,  C.  Boosting  reverse intersystem  crossing  by  increasing  donors  in  triarylboron/phenoxazine  hybrids:  TADF  emitters  for high-performance solution-processed OLEDs. Journal of Materials Chemistry C 2016 , 4 , 4402-4407.
- 27. Tang, C.; Yang, T.; Cao, X.; Tao, Y.; Wang, F.; Zhong, C.; Qian, Y.; Zhang, X.; Huang, W. Tuning a Weak Emissive Blue Host to Highly Efficient Green Dopant by a CN in Tetracarbazolepyridines for SolutionProcessed Thermally Activated Delayed Fluorescence Devices. Advanced Optical Materials 2015 , 3 , 786790, doi:doi:10.1002/adom.201500016.
- 28. Chen, X.-L.; Lin, C.-S.; Wu, X.-Y.; Yu, R.; Teng, T.; Zhang, Q.-K.; Zhang, Q.; Yang, W.-B.; Lu, C.-Z. Highly efficient  cuprous  complexes  with  thermally  activated  delayed  fluorescence  and  simplified  solution process  OLEDs  using  the  ligand  as  host. Journal  of  Materials  Chemistry  C 2015 , 3 , 1187-1195, doi:10.1039/C4TC02255F.
- 29. Joo,  C.W.;  Cho,  H.;  Kwon,  B.-H.;  Cho,  N.S.;  Kim,  Y.;  Kim,  Y.-H.;  Lee,  J.  Development  of  solutionprocessable blue/hybrid-white OLEDs based on thermally activated delayed fluorescence. Journal of Industrial and Engineering Chemistry 2018 , 65 , 35-39, doi:https://doi.org/10.1016/j.jiec.2018.03.030.

- 30. Li, W.; Zhao, J.; Li, L.; Du, X.; Fan, C.; Zheng, C.; Tao, S. Efficient solution-processed blue and white OLEDs based on a high-triplet bipolar host and a blue TADF emitter. Organic Electronics 2018 , 58 , 276282, doi:https://doi.org/10.1016/j.orgel.2018.04.027.
- 31. Luo, J.; Gong, S.; Gu, Y.; Chen, T.; Li, Y.; Zhong, C.; Xie, G.; Yang, C. Multi-carbazole encapsulation as a simple strategy for the construction of solution-processed, non-doped thermally activated delayed fluorescence emitters. Journal of Materials Chemistry C 2016 , 4 , 2442-2446, doi:10.1039/C6TC00418K.

32.

- a thermally activated delayed fluorescence emitter. Synthetic Metals 2015 , 202 , doi:https://doi.org/10.1016/j.synthmet.2015.02.009.
- Komatsu, R.; Sasabe, H.; Inomata, S.; Pu, Y.-J.; Kido, J. High efficiency solution processed OLEDs using 165-168,
- 33. Luo, J.; Xie, G.; Gong, S.; Chen, T.; Yang, C. Creating a thermally activated delayed fluorescence channel in a single polymer system to enhance exciton utilization efficiency for bluish-green electroluminescence. Chemical Communications 2016 , 52 , 2292-2295, doi:10.1039/C5CC09797E.
- 34. Cho,  Y.J.;  Jeon,  S.K.;  Lee,  J.Y.  Molecular  Engineering  of  High  Efficiency  and  Long  Lifetime  Blue Thermally Activated Delayed Fluorescent Emitters for Vacuum and Solution Processed Organic LightEmitting Diodes. Advanced Optical Materials 2016 , 4 , 688-693, doi:doi:10.1002/adom.201500634.
- 35. Kim, Y.-H.; Wolf, C.; Cho, H.; Jeong, S.-H.; Lee, T.-W. Highly Efficient, Simplified, Solution-Processed Thermally Activated Delayed-Fluorescence Organic Light-Emitting Diodes. Advanced Materials 2016 , 28 , 734-741, doi:doi:10.1002/adma.201504490.
- 36. Nobuyasu, R.S.; Ren, Z.; Griffiths, G.C.; Batsanov, A.S.; Data, P.; Yan, S.; Monkman, A.P.; Bryce, M.R.; Dias, F.B. Rational Design of TADF Polymers Using a Donor-Acceptor Monomer with Enhanced TADF Efficiency  Induced  by  the  Energy  Alignment  of  Charge  Transfer  and  Local  Triplet  Excited  States. Advanced Optical Materials 2016 , 4 , 597-607, doi:doi:10.1002/adom.201500689.
- 37. Sun, K.; Sun, Y.; Huang, T.; Luo, J.; Jiang, W.; Sun, Y. Design strategy of yellow thermally activated delayed fluorescent dendrimers and their highly efficient non-doped solution-processed OLEDs with low driving voltage. Organic Electronics 2017 , 42 , 123-130, doi:https://doi.org/10.1016/j.orgel.2016.12.026.
- 38. Ban, X.; Jiang, W.; Sun, K.; Lin, B.; Sun, Y. Self-Host Blue Dendrimer Comprised of Thermally Activated Delayed  Fluorescence  Core  and  Bipolar  Dendrons  for  Efficient  Solution-Processable  Nondoped Electroluminescence. ACS Applied Materials &amp; Interfaces 2017 , 9 , 7339-7346, doi:10.1021/acsami.6b14922.
- 39. Hu, J.; Zhang, X.; Zhang, D.; Cao, X.; Jiang, T.; Zhang, X.; Tao, Y. Linkage modes  on phthaloyl/triphenylamine hybrid compounds: Multi-functional AIE luminogens, non-doped emitters and  organic  hosts  for  highly  efficient  solution-processed  delayed  fluorescence  OLEDs. Dyes  and Pigments 2017 , 137 , 480-489, doi:https://doi.org/10.1016/j.dyepig.2016.10.029.
- 40. Ban, X.; Zhu, A.; Zhang, T.; Tong, Z.; Jiang, W.; Sun, Y. Design of encapsulated hosts and guests for highly efficient blue and green thermally activated delayed fluorescence OLEDs based on a solutionprocess. Chemical Communications 2017 , 53 , 11834-11837.
- 41. Gong, S.; Luo, J.; Wang, Z.; Li, Y.; Chen, T.; Xie, G.; Yang, C. Tuning emissive characteristics and singlettriplet  energy  splitting  of  fluorescent  emitters  by  encapsulation  group  modification:  Yellow  TADF emitter for solution-processed OLEDs with high luminance and ultraslow efficiency roll-off. Dyes and Pigments 2017 , 139 , 593-600, doi:https://doi.org/10.1016/j.dyepig.2016.12.058.
- 42. Bin, H.; Ji, Y.; Li, Z.; Zhou, N.; Jiang, W.; Feng, Y.; Lin, B.; Sun, Y. Simple aggregation-induced delayed fluorescence materials based on anthraquinone derivatives for highly efficient solution-processed red OLEDs. Journal of Luminescence 2017 , 187 , 414-420, doi:https://doi.org/10.1016/j.jlumin.2017.03.038.

- 43. Huang,  B.;  Li,  Z.;  Yang,  H.;  Hu,  D.;  Wu,  W.;  Feng,  Y.;  Sun,  Y.;  Lin,  B.;  Jiang,  W.  Bicolour electroluminescence of 2-(carbazol-9-yl)anthraquinone based on a solution process. Journal of Materials Chemistry C 2017 , 5 , 12031-12034, doi:10.1039/C7TC04444E.
- 44. Huang, B.; Ban, X.; Sun, K.; Ma, Z.; Mei, Y.; Jiang, W.; Lin, B.; Sun, Y. Thermally activated delayed fluorescence materials based on benzophenone derivative as emitter for efficient solution-processed non-doped green OLED. Dyes and Pigments 2016 , 133 , 380-386, doi:https://doi.org/10.1016/j.dyepig.2016.06.025.
- 45. Lin, X.; Zhu, Y.; Zhang, B.; Zhao, X.; Yao, B.; Cheng, Y.; Li, Z.; Qu, Y.; Xie, Z. Highly Efficient TADF Polymer Electroluminescence with Reduced Efficiency Roll-off via Interfacial Exciplex Host Strategy. ACS Applied Materials &amp; Interfaces 2018 , 10 , 47-52, doi:10.1021/acsami.7b16887.
- 46. Zhu, Y.; Zhang, Y.; Yao, B.; Wang, Y.; Zhang, Z.; Zhan, H.; Zhang, B.; Xie, Z.; Wang, Y.; Cheng, Y. Synthesis  and  Electroluminescence  of  a  Conjugated  Polymer  with  Thermally  Activated  Delayed Fluorescence. Macromolecules 2016 , 49 , 4373-4377, doi:10.1021/acs.macromol.6b00430.
- 47. Cho, Y.J.; Chin, B.D.; Jeon, S.K.; Lee, J.Y. 20% External Quantum Efficiency in Solution-Processed Blue Thermally Activated Delayed Fluorescent Devices. Advanced Functional Materials 2015 , 25 , 6786-6792, doi:doi:10.1002/adfm.201502995.
- 48. Li, Y.; Xie, G.; Gong, S.; Wu, K.; Yang, C. Dendronized delayed fluorescence emitters for non-doped, solution-processed  organic  light-emitting  diodes  with  high  efficiency  and  low  efficiency  roll-off simultaneously: two parallel emissive channels. Chemical Science 2016 , 7 , 5441-5447, doi:10.1039/C6SC00943C.
- 49. Yu, L.; Wu, Z.; Xie, G.; Zhong, C.; Zhu, Z.; Cong, H.; Ma, D.; Yang, C. Achieving a balance between small  singlet-triplet  energy  splitting  and  high  fluorescence  radiative  rate  in  a  quinoxaline-based orange-red thermally activated delayed fluorescence emitter. Chemical Communications 2016 , 52 , 1101211015, doi:10.1039/C6CC05203G.
- 50. Ban, X.; Jiang, W.; Lu, T.; Jing, X.; Tang, Q.; Huang, S.; Sun, K.; Huang, B.; Lin, B.; Sun, Y. Self-host thermally activated delayed fluorescent dendrimers with flexible chains: an effective strategy for nondoped electroluminescent devices based on solution processing. Journal of Materials Chemistry C 2016 , 4 , 8810-8816, doi:10.1039/C6TC03063G.
- 51. Li,  J.;  Liao,  X.;  Xu,  H.;  Li,  L.;  Zhang,  J.;  Wang,  H.;  Xu,  B.  Deep-blue  thermally  activated  delayed fluorescence dendrimers with reduced singlet-triplet energy gap for low roll-off non-doped solutionprocessed organic light-emitting diodes. Dyes and Pigments 2017 , 140 , 79-86, doi:https://doi.org/10.1016/j.dyepig.2017.01.036.
- 52. Matsuoka, K.; Albrecht, K.; Yamamoto, K.; Fujita, K. Mulifunctional Dendritic Emitter: AggregationInduced  Emission  Enhanced,  Thermally  Activated  Delayed  Fluorescent  Material  for  SolutionProcessed Multilayered Organic Light-Emitting Diodes. Scientific Reports 2017 , 7 , 41780, doi:10.1038/srep41780

## https://www.nature.com/articles/srep41780#supplementary-information.

- 53. Sun,  K.;  Xie,  X.;  Liu,  Y.;  Jiang,  W.;  Ban,  X.;  Huang,  B.;  Sun,  Y.  Thermally  cross-linkable  thermally activated  delayed  fluorescent  materials  for  efficient  blue  solution-processed  organic  light-emitting diodes. Journal of Materials Chemistry C 2016 , 4 , 8973-8979, doi:10.1039/C6TC02634F.
- 54. Verma, A.; Zink, D.M.; Fléchon, C.; Leganés Carballo, J.; Flügge, H.; Navarro, J.M.; Baumann, T.; Volz, D. Efficient, inkjet-printed TADF-OLEDs with an ultra-soluble NHetPHOS complex. Applied Physics A 2016 , 122 , 191, doi:10.1007/s00339-016-9726-2.

- 55. Chen, X.-L.; Yu, R.; Zhang, Q.-K.; Zhou, L.-J.; Wu, X.-Y.; Zhang, Q.; Lu, C.-Z. Rational Design of Strongly Blue-Emitting Cuprous Complexes with Thermally Activated Delayed Fluorescence and Application in Solution-Processed OLEDs. Chemistry of Materials 2013 , 25 , 3910-3920, doi:10.1021/cm4024309.
- 56. Chen, X.-L.; Jia, J.-H.; Yu, R.; Liao, J.-Z.; Yang, M.-X.; Lu, C.-Z. Combining Charge-Transfer Pathways to Achieve  Unique  Thermally  Activated  Delayed  Fluorescence  Emitters  for  High-Performance Solution-Processed, Non-doped Blue OLEDs. 2017 , 56 , 15006-15009, doi:doi:10.1002/anie.201709125.
- 57. Ban,  X.;  Zhu,  A.;  Zhang,  T.;  Tong,  Z.;  Jiang,  W.;  Sun,  Y.  Highly  Efficient  All-Solution-Processed Fluorescent Organic Light-Emitting Diodes Based on a Novel Self-Host Thermally Activated Delayed Fluorescence Emitter. ACS Applied Materials &amp; Interfaces 2017 , 9 , 21900-21908, doi:10.1021/acsami.7b04146.
- 58. Nikolaenko,  A.E.;  Cass,  M.;  Bourcet,  F.;  Mohamad,  D.;  Roberts,  M.  Thermally  Activated  Delayed Fluorescence  in  Polymers:  A  New  Route  toward  Highly  Efficient  Solution  Processable  OLEDs. Advanced Materials 2015 , 27 , 7236-7240, doi:doi:10.1002/adma.201501090.
- 59. Ren, Z.; Nobuyasu, R.S.; Dias, F.B.; Monkman, A.P.; Yan, S.; Bryce, M.R. Pendant Homopolymer and Copolymers as Solution-Processable Thermally Activated Delayed Fluorescence Materials for Organic Light-Emitting Diodes. Macromolecules 2016 , 49 , 5452-5460, doi:10.1021/acs.macromol.6b01216.
- 60. Xie, G.; Luo, J.; Huang, M.; Chen, T.; Wu, K.; Gong, S.; Yang, C. Inheriting the Characteristics of TADF Small  Molecule  by  Side-Chain  Engineering  Strategy  to  Enable  Bluish-Green  Polymers  with  High PLQYs up to  74% and  External  Quantum  Efficiency  over  16%  in  Light-Emitting  Diodes. Advanced Materials 2017 , 29 , 1604223, doi:doi:10.1002/adma.201604223.
- 61. Dias, F.B.; Bourdakos, K.N.; Jankus, V.; Moss, K.C.; Kamtekar, K.T.; Bhalla, V.; Santos, J.; Bryce, M.R.; Monkman, A.P.  Triplet  Harvesting  with  100%  Efficiency  by  Way  of  Thermally  Activated  Delayed Fluorescence in Charge Transfer OLED Emitters. Advanced Materials 2013 , 25 , 3707-3714, doi:doi:10.1002/adma.201300753.
- 62. Kim, K.-H.; Lee, S.; Moon, C.-K.; Kim, S.-Y.; Park, Y.-S.; Lee, J.-H.; Woo Lee, J.; Huh, J.; You, Y.; Kim, J.J. Phosphorescent dye-based supramolecules for high-efficiency organic light-emitting diodes. 2014 , 5 , 4769, doi:10.1038/ncomms5769

## https://www.nature.com/articles/ncomms5769#supplementary-information.

- 63. Flämmich, M.; Frischeisen, J.; Setz, D.S.; Michaelis, D.; Krummacher, B.C.; Schmidt, T.D.; Brütting, W.; Danz, N. Oriented phosphorescent emitters boost OLED efficiency. Organic Electronics 2011 , 12 , 16631668, doi:https://doi.org/10.1016/j.orgel.2011.06.011.
- 64. Facchetti,  A.  π -Conjugated  polymers  for  organic  electronics  and  photovoltaic  cell  applications. Chemistry of Materials 2010 , 23 , 733-758.
- 65. Salaneck, W.R.; Stafstrom, S.; Brédas, J.L. Conjugated polymer surfaces and interfaces: electronic and chemical structure of interfaces for polymer light emitting devices ; Cambridge University Press: 2003.
- 66. Lee,  J.;  Aizawa,  N.;  Numata,  M.;  Adachi,  C.;  Yasuda,  T.  Versatile  molecular  functionalization  for inhibiting  concentration  quenching  of  thermally  activated  delayed  fluorescence. Advanced  Materials 2017 , 29 , 1604856.
- 67. Xie, Z.; Chen, C.; Xu, S.; Li, J.; Zhang, Y.; Liu, S.; Xu, J.; Chi, Z. White-Light Emission Strategy of a Single Organic  Compound  with  Aggregation-Induced  Emission  and  Delayed  Fluorescence  Properties. Angewandte Chemie International Edition 2015 , 54 , 7181-7184.
- 68. Song, W.; Lee, I.; Lee, J.Y. Host Engineering for High Quantum Efficiency Blue and White Fluorescent Organic Light-Emitting Diodes. Advanced Materials 2015 , 27 , 4358-4363.

- 69. Cho, Y.J.; Yook, K.S.; Lee, J.Y. High Efficiency in a Solution-Processed Thermally Activated DelayedFluorescence  Device  Using  a  Delayed-Fluorescence  Emitting  Material  with  Improved  Solubility. Advanced Materials 2014 , 26 , 6642-6646.
- 70. Suzuki, Y.; Zhang, Q.; Adachi, C. A solution-processable host material of 1, 3-bis {3-[3-(9-carbazolyl) phenyl]-9-carbazolyl} benzene and its application in organic light-emitting diodes employing thermally activated delayed fluorescence. Journal of Materials Chemistry C 2015 , 3 , 1700-1706.
- 71. Kim, J.-S.; Friend, R.H.; Grizzi, I.; Burroughes, J.H. Spin-cast thin semiconducting polymer interlayer for  improving  device  efficiency  of  polymer  light-emitting  diodes. Applied  Physics  Letters 2005 , 87 , 023506.
- 72. Tsujimoto, H.; Ha, D.-G.; Markopoulos, G.; Chae, H.S.; Baldo, M.A.; Swager, T.M. Thermally Activated Delayed  Fluorescence  and  Aggregation  Induced  Emission  with  Through-Space  Charge  Transfer. Journal of the American Chemical Society 2017 , 139 , 4894-4900, doi:10.1021/jacs.7b00873.
- 73. Feuillastre, S.; Pauton, M.; Gao, L.; Desmarchelier, A.; Riives, A.J.; Prim, D.; Tondelier, D.; Geffroy, B.; Muller, G.; Clavier, G., et al. Design and Synthesis of New Circularly Polarized Thermally Activated Delayed Fluorescence Emitters. J Am Chem Soc 2016 , 138 , 3990-3993, doi:10.1021/jacs.6b00850.
- 74. Mei, J.; Leung, N.L.C.; Kwok, R.T.K.; Lam, J.W.Y.; Tang, B.Z. Aggregation-Induced Emission: Together We Shine, United We Soar! Chemical Reviews 2015 , 115 , 11718-11940, doi:10.1021/acs.chemrev.5b00263.
- 75. Li, J.; Liu, D. Dendrimers for organic light-emitting diodes. Journal of materials Chemistry 2009 , 19 , 75847591.
- 76. Lo,  S.-C.;  Burn,  P.L.  Development  of  dendrimers:  macromolecules  for  use  in  organic  light-emitting diodes and solar cells. Chemical Reviews 2007 , 107 , 1097-1116.
- 77. Albrecht,  K.;  Pernites,  R.;  Felipe, M.J.; Advincula,  R.C.;  Yamamoto,  K.  Patterning  CarbazolePhenylazomethine Dendrimer Films. Macromolecules 2012 , 45 , 1288-1295, doi:10.1021/ma202485h.
- 78. Kimoto, A.; Cho, J.-S.; Ito, K.; Aoki, D.; Miyake, T.; Yamamoto, K. Novel Hole-Transport Material for Efficient Polymer Light-Emitting Diodes by Photoreaction. Macromolecular Rapid Communications 2005 , 26 , 597-601, doi:doi:10.1002/marc.200400657.
- 79. Aizawa, N.; Pu, Y.-J.; Watanabe, M.; Chiba, T.; Ideta, K.; Toyota, N.; Igarashi, M.; Suzuri, Y.; Sasabe, H.; Kido,  J.  Solution-processed  multilayer  small-molecule  light-emitting  devices  with  high-efficiency white-light emission. Nature Communications 2014 , 5 , 5756, doi:10.1038/ncomms6756

## https://www.nature.com/articles/ncomms6756#supplementary-information.

- 80. Chen, L.; Ma, Z.; Ding, J.; Wang, L.; Jing, X.; Wang, F. Self-host heteroleptic green iridium dendrimers: achieving  efficient  non-doped  device  performance  based  on  a  simple  molecular  structure. Chemical Communications 2011 , 47 , 9519-9521, doi:10.1039/C1CC13276H.
- 81. Leijtens,  T.;  Ding,  I.-K.;  Giovenzana,  T.;  Bloking,  J.T.;  McGehee,  M.D.;  Sellinger,  A.  Hole  transport materials with low glass transition temperatures and high solubility for application in solid-state dyesensitized solar cells. ACS nano 2012 , 6 , 1455-1462.
- 82. Hansen, C.M. The three dimensional solubility parameter. Danish Technical: Copenhagen 1967 , 14 .
- 83. Barton, A.F. Solubility parameters. Chemical Reviews 1975 , 75 , 731-753.
- 84. Machui, F.; Abbott, S.; Waller, D.; Koppe, M.; Brabec, C.J. Determination of solubility parameters for organic semiconductor formulations. Macromolecular chemistry and Physics 2011 , 212 , 2159-2165.
- 85. Burgués-Ceballos, I.; Machui, F.; Min, J.; Ameri, T.; Voigt, M.M.; Luponosov, Y.N.; Ponomarenko, S.A.; Lacharmoise, P.D.; Campoy-Quiles, M.; Brabec, C.J. Solubility based identification of green solvents for small molecule organic solar cells. Advanced Functional Materials 2014 , 24 , 1449-1457.

- 86. Machui, F.; Langner, S.; Zhu, X.; Abbott, S.; Brabec, C.J. Determination of the P3HT:PCBM solubility parameters via a binary solvent gradient method: Impact of solubility on the photovoltaic performance. Solar Energy Materials and Solar Cells 2012 , 100 , 138-146, doi:https://doi.org/10.1016/j.solmat.2012.01.005.
- 87. Duong, D.T.; Walker, B.; Lin, J.; Kim, C.; Love, J.; Purushothaman, B.; Anthony, J.E.; Nguyen, T.Q. Molecular  solubility  and  hansen  solubility  parameters  for  the  analysis  of  phase  separation  in  bulk heterojunctions. Journal of Polymer Science Part B: Polymer Physics 2012 , 50 , 1405-1413.
- 88. Sanders, J.M.; Kwak, H.S.; Mustard, T.J.; Browning, A.R.; Halls, M.D. Atomistic simulations of mechanical and thermophysical properties of OLED materials ; SPIE: 2018; Vol. 10736, pp. 8.
- 89. Kamyshny, A.; Magdassi, S. Conductive Nanomaterials for Printed Electronics. Small 2014 , 10 , 35153535, doi:doi:10.1002/smll.201303000.
- 90. Ankireddy,  K.;  Vunnam,  S.;  Kellar,  J.;  Cross,  W.  Highly  conductive  short  chain  carboxylic  acid encapsulated silver nanoparticle based inks for direct write technology applications. Journal of Materials Chemistry C 2013 , 1 , 572-579, doi:10.1039/C2TC00336H.
- 91. Vaseem, M.; Lee, K.M.; Hong, A.R.; Hahn, Y.-B. Inkjet Printed Fractal-Connected Electrodes with Silver Nanoparticle Ink. ACS Applied Materials &amp; Interfaces 2012 , 4 , 3300-3307, doi:10.1021/am300689d.
- 92. Yamada, T.; Fukuhara, K.; Matsuoka, K.; Minemawari, H.; Tsutsumi, J.y.; Fukuda, N.; Aoshima, K.; Arai, S.; Makita, Y.; Kubo, H., et al. Nanoparticle chemisorption printing technique for conductive silver patterning with submicron resolution. Nature Communications 2016 , 7 , 11402, doi:10.1038/ncomms11402

## https://www.nature.com/articles/ncomms11402#supplementary-information.

- 93. Wu,  Y.;  Li,  Y.;  Ong,  B.S.;  Liu,  P.;  Gardner,  S.;  Chiang,  B.  High-Performance  Organic  Thin-Film Transistors with Solution-Printed Gold Contacts. Advanced Materials 2005 , 17 , 184-187, doi:doi:10.1002/adma.200400690.
- 94. Jung, S.-h.; Choi, D.Y.; Lee, H.M. Roll-to-roll processed, highly conductive, and flexible aluminum (Al) electrodes based on Al precursor inks. RSC Advances 2018 , 8 , 19950-19957, doi:10.1039/C8RA03303J.
- 95. Lee, H.M.; Seo, J.Y.; Jung, A.; Choi, S.-Y.; Ko, S.H.; Jo, J.; Park, S.B.; Park, D. Long-Term Sustainable Aluminum Precursor Solution for Highly Conductive Thin Films on Rigid and Flexible Substrates. ACS Applied Materials &amp; Interfaces 2014 , 6 , 15480-15487, doi:10.1021/am504134f.
- 96. Chang, J.-H.; Lin, W.-H.; Wang, P.-C.; Taur, J.-I.; Ku, T.-A.; Chen, W.-T.; Yan, S.-J.; Wu, C.-I. Solutionprocessed transparent blue organic light-emitting diodes with graphene as the top cathode. Scientific reports 2015 , 5 , 9693.
- 97. Matyba, P.; Yamaguchi, H.; Eda, G.; Chhowalla, M.; Edman, L.; Robinson, N.D. Graphene and mobile ions: the key to all-plastic, solution-processed light-emitting devices. Acs Nano 2010 , 4 , 637-642.
- 98. Wang, J.; Liu, L.; Ling, Z.; Yang, J.; Wan, C.; Jiang, C. Polymer lithium cells with sulfur composites as cathode materials. Electrochimica Acta 2003 , 48 , 1861-1867, doi:https://doi.org/10.1016/S00134686(03)00258-5.
- 99. Kim, J.-K.;  Cheruvally, G.; Choi, J.-W.; Ahn, J.-H.; Lee, S.H.; Choi, D.S.; Song, C.E. Effect of radical polymer cathode thickness on the electrochemical performance of organic radical battery. Solid State Ionics 2007 , 178 , 1546-1551, doi:https://doi.org/10.1016/j.ssi.2007.09.009.
- 100. Novák, P.; Müller, K.; Santhanam, K.S.V.; Haas, O. Electrochemically Active Polymers for Rechargeable Batteries. Chemical Reviews 1997 , 97 , 207-282, doi:10.1021/cr941181o.
- 101. Song,  Z.;  Zhan,  H.;  Zhou,  Y.  Polyimides:  Promising  Energy-Storage  Materials. Angewandte  Chemie International Edition 2010 , 49 , 8444-8448, doi:doi:10.1002/anie.201002439.

̈

|   102. | Oyama, N.; Tatsuma, T.; Sato, T.; Sotomura, T. Dimercaptan-polyaniline composite electrodes for lithium batteries with high energy density. Nature 1995 , 373 , 598-600, doi:10.1038/373598a0.                                                                                                                                        |
|--------|---------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------------|
|    103 | Peterson, B.M.; Ren, D.; Shen, L.; Wu, Y.-C.M.; Ulgut, B.; Coates, G.W.; Abruña, H.D.; Fors, B.P. Phenothiazine-Based Polymer Cathode Materials with Ultrahigh Power Densities for Lithium Ion Batteries. ACS Applied Energy Materials 2018 , 1 , 3560-3564.                                                                          |
|    104 | Suga, T.; Konishi, H.; Nishide, H. Photocrosslinked nitroxide polymer cathode-active materials for application in an organic-based paper battery. Chemical Communications 2007 , 10.1039/B618710B, 1730- 1732, doi:10.1039/B618710B.                                                                                                  |
|    105 | Gadisa, A.; Tvingstedt, K.; Admassie, S.; Lindell, L.; Crispin, X.; Andersson, M.R.; Salaneck, W.R.; Inganäs, O. Transparent polymer cathode for organic photovoltaic devices. Synthetic Metals 2006 , 156 , 1102-1107.                                                                                                               |
|    106 | Godumala, M.; Choi, S.; Cho, M.J.; Choi, D.H. Recent breakthroughs in thermally activated delayed fluorescence organic light emitting diodes containing non-doped emitting layers. Journal of Materials Chemistry C 2019 , 10.1039/C8TC06293E, doi:10.1039/C8TC06293E.                                                                |
|    107 | Angioni, E.; Chapran, M.; Ivaniuk, K.; Kostiv, N.; Cherpak, V.; Stakhira, P.; Lazauskas, A.; Tamulevičius, S.; Volyniuk, D.; Findlay, N. A single emitting layer white OLED based on exciplex interface emission. Journal of Materials Chemistry C 2016 , 4 , 3851-3856.                                                              |
|    108 | Feng, X.J.; Chen, S.F.; Ni, Y.; Wong, M.S.; Lam, M.M.; Cheah, K.W.; Lai, G.Q. Fluorene derivatives for highly efficient non-doped single-layer blue organic light-emitting diodes. Organic Electronics 2014 , 15 , 57-64.                                                                                                             |
|    109 | Meier, S.B.; Tordera, D.; Pertegas, A.; Roldan-Carmona, C.; Ortí, E.; Bolink, H.J. Light-emitting electrochemical cells: recent progress and future prospects. Materials Today 2014 , 17 , 217-223.                                                                                                                                   |
|    110 | Pertegás, A.; Wong, M.Y.; Sessolo, M.; Zysman-Colman, E.; Bolink, H.J. Efficient Light-Emitting Electrochemical Cells Using Small Molecular Weight, Ionic, Host-Guest Systems. ECS Journal of Solid State Science and Technology 2016 , 5 , R3160-R3163, doi:10.1149/2.0201601jss.                                                    |
|    111 | Wong, M.Y.; La-Placa, M.-G.; Pertegas, A.; Bolink, H.J.; Zysman-Colman, E. Deep-blue thermally activated delayed fluorescence (TADF) emitters for light-emitting electrochemical cells (LEECs). Journal of Materials Chemistry C 2017 , 5 , 1699-1705.                                                                                |
|    112 | Wong, M.Y.; Hedley, G.J.; Xie, G.; Kolln, L.S.; Samuel, I.D.; Perteg á s, A.; Bolink, H.J.; Zysman-Colman, E. Light-emitting electrochemical cells and solution-processed organic light-emitting diodes using small molecule organic thermally activated delayed fluorescence emitters. Chemistry of Materials 2015 , 27 , 6535-6542. |
|    113 | Wong, M.Y.; Zysman-Colman, E. Thermally Activated Delayed Fluorescence Emitters in Light- Emitting Electrochemical Cells. In Light-Emitting Electrochemical Cells: Concepts, Advances and Challenges , Costa, R.D., Ed. Springer International Publishing: Cham, 2017; 10.1007/978-3-319-58613-7_9pp. 237-                            |
Sahadev Somasundaram
Solution Processability and Thermally Activated Delayed Fluorescence: Two Steps towards Low-Cost Organic Light Emitting Diodes
Organic Light Emitting Diodes (OLED) have experienced vast attention in the
scientific literature as the leading contender for the next generation of
electronic lighting technology. However, while research continues to push the
limit for OLED performance and efficiencies, minimal attention is paid to the
processability and suitability for mass production. In this regard, Solution
Processability (SP) and Thermally Activated Delayed Fluorescence (TADF) in
OLEDs are two recent discoveries which have significantly improved the capacity
for low-cost processing without compromise to their performance efficiencies.
This meta-analysis is focused on these discoveries and their application to
OLEDs. Recent peer-reviewed studies of OLEDs employing both SP and TADF are
reviewed in order to highlight physical fundamentals and discover synergistic
effects when incorporating both factors into a single OLED device.
Additionally, some other recent trends targeting efficient manufacturing of
OLEDs are identified, and logical future directions for interested researchers
are discussed.